## 3 Results and Discussion
### Analysis of Deposited Zinc Mass and Zinc Coating Quality
#### 3.2.1 Electrolytic Zinc Coating  
In the context of electrolytic deposition, ref. [30] states that the deposition rate of the coating metal generally depends not only on the microstructure of the substrate but also on the temperature of the plating bath (electrolyte). Furthermore, ref. [31] adds that increasing the bath temperature enhances electrical conductivity, thereby accelerating metal transfer to the substrate. However, since all electroplating experiments in this study were conducted at a constant electrolyte temperature of 25 \(\pm\) 1 \({}^{\circ}\)C, the influence of temperature on the zinc deposition rate can be considered negligible in this case. Regardless of the  
\begin{table} \begin{tabular}{c c c c c c} \hline \hline
**Type of MP** & \multicolumn{4}{c}{**Electrolytic Zinc Deposition Time (s)**} \\ \hline  & **900** & **1800** & **2700** & **2600** & **4500** \\ \hline SCB & 33.62 \(\pm\) 0.71 & 59.48 \(\pm\) 0.97 & 81.93 \(\pm\) 1.22 & 102.59 \(\pm\) 1.57 & 116.45 \(\pm\) 1.96 \\ SGB & 28.72 \(\pm\) 0.49 & 52.13 \(\pm\) 0.70 & 69.88 \(\pm\) 0.92 & 87.47 \(\pm\) 0.99 & 96.27 \(\pm\) 1.16 \\ G & 30.97 \(\pm\) 0.52 & 55.46 \(\pm\) 0.74 & 72.44 \(\pm\) 0.89 & 90.23 \(\pm\) 1.02 & 102.45 \(\pm\) 1.19 \\ E & 24.21 \(\pm\) 0.39 & 43.18 \(\pm\) 0.57 & 60.53 \(\pm\) 0.71 & 75.14 \(\pm\) 0.83 & 78.80 \(\pm\) 0.87 \\ \hline \hline \end{tabular} \begin{tabular}{c c c c c} \hline \hline
**Type of MP** & \multicolumn{4}{c}{**Hot-Dip Zinc Deposition Time (s)**} \\ \hline  & **70** & **105** & **140** & **175** & **210** \\ \hline SCB & 164.17 \(\pm\) 3.77 & 278.24 \(\pm\) 5.29 & 356.32 \(\pm\) 6.73 & 439.84 \(\pm\) 8.02 & 507.91 \(\pm\) 9.81 \\ SGB & 145.85 \(\pm\) 2.93 & 242.80 \(\pm\) 4.36 & 326.37 \(\pm\) 5.87 & 409.58 \(\pm\) 7.39 & 458.44 \(\pm\) 8.23 \\ G & 209.83 \(\pm\) 3.94 & 297.51 \(\pm\) 5.07 & 368.74 \(\pm\) 5.98 & 424.69 \(\pm\) 6.78 & 477.13 \(\pm\) 7.87 \\ E & 184.39 \(\pm\) 3.31 & 266.89 \(\pm\) 4.17 & 334.28 \(\pm\) 4.80 & 393.95 \(\pm\) 5.53 & 442.21 \(\pm\) 6.09 \\ \hline \hline \end{tabular} \begin{tabular}{c c c c c} \hline \hline
**Type of MP** & \multicolumn{4}{c}{**Electrolytic Zinc Deposition Time (s)**} \\ \hline  & **900** & **1800** & **2700** & **2600** & **4500** \\ \hline SCB & 33.62 \(\pm\) 0.71 & 59.48 \(\pm\) 0.97 & 81.93 \(\pm\) 1.22 & 102.59 \(\pm\) 1.57 & 116.45 \(\pm\) 1.96 \\ SGB & 28.72 \(\pm\) 0.49 & 52.13 \(\pm\) 0.70 & 69.88 \(\pm\) 0.92 & 87.47 \(\pm\) 0.99 & 96.27 \(\pm\) 1.16 \\ G & 30.97 \(\pm\) 0.52 & 55.46 \(\pm\) 0.74 & 72.44 \(\pm\) 0.89 & 90.23 \(\pm\) 1.02 & 102.45 \(\pm\) 1.19 \\ E & 24.21 \(\pm\) 0.39 & 43.18 \(\pm\) 0.57 & 60.53 \(\pm\) 0.71 & 75.14 \(\pm\) 0.83 & 78.80 \(\pm\) 0.87 \\ \hline \hline \end{tabular} \begin{tabular}{c c c c c} \hline \hline
**Type of MP** & \multicolumn{4}{c}{**Hot-Dip Zinc Deposition Time (s)**} \\ \hline  & **70** & **105** & **140** & **175** & **210** \\ \hline SCB & 164.17 \(\pm\) 3.77 & 278.24 \(\pm\) 5.29 & 356.32 \(\pm\) 6.73 & 439.84 \(\pm\) 8.02 & 507.91 \(\pm\) 9.81 \\ SGB & 145.85 \(\pm\) 2.93 & 242.80 \(\pm\) 4.36 & 326.37 \(\pm\) 5.87 & 409.58 \(\pm\) 7.39 & 458.44 \(\pm\) 8.23 \\ G & 209.83 \(\pm\) 3.94 & 297.51 \(\pm\) 5.07 & 368.74 \(\pm\) 5.98 & 424.69 \(\pm\) 6.78 & 477.13 \(\pm\) 7.87 \\ E & 184.39 \(\pm\) 3.31 & 266.89 \(\pm\) 4.17 & 334.28 \(\pm\) 4.80 & 393.95 \(\pm\) 5.53 & 442.21 \(\pm\) 6.09 \\ \hline \hline \end{tabular}